Experimental Study and Modelling of Plastic Deformation of ... deformation rate, and the resulting...
Embed Size (px)
Transcript of Experimental Study and Modelling of Plastic Deformation of ... deformation rate, and the resulting...
Procedia CIRP 14 ( 2014 ) 599 – 604
Available online at www.sciencedirect.com
2212-8271 © 2014 Published by Elsevier B.V. Open access under CC BY-NC-ND license. Selection and peer-review under responsibility of the International Scientific Committee of the 6th CIRP International Conference on High Performance Cutting doi: 10.1016/j.procir.2014.03.021
6th CIRP International Conference on High Performance Cutting, HPC2014
Experimental Study and Modelling of Plastic Deformation of Cemented Carbide Tools in Turning
Anders Nordgrena*, Baktash Zargari Samanib, Rachid M´Saoubic a Sandvik Coromant AB, Stockholm, Sweden
b Sandvik SRP AB, Svedala, Sweden c Seco Tools AB, Fagersta, Sweden
* Corresponding author. Tel.: +46-70-6696608; fax: +46-8-7266561. E-mail address: email@example.com
The plastic deformation of coated cemented carbide cutting tools was investigated. Testing methods were developed for the experimental determination of the high-temperature strength of cemented carbide (compressive strength, creep resistance). CVD-coated cemented carbide inserts were tested in continuous turning of quenched and tempered steel (AISI 4340). Cutting forces and edge temperature distributions were measured in 2D orthogonal turning. Normal stress distributions on the tool surface were estimated from measured cutting forces and tool-chip contact lengths. These data, together with measured high-temperature strength data for the cemented carbide, were introduced into a finite element model (ANSYS). The agreement between the predicted deformation and the experimental results was acceptable. The difference between the simulated and measured flank width on deformed cutting edges was approximately 15%. It has been demonstrated that numerical methods (FE) provide an opportunity to describe the effect of cutting conditions and tool material properties on tool behaviour quantitatively and in a systematic manner.
© 2014 The Authors. Published by Elsevier B.V. Selection and peer-review under responsibility of the International Scientific Committee of the 6th CIRP International Conference on High Performance Cutting.
Keywords: Cemented carbide; compressive strength; creep; metal cutting; turning; plastic deformation, cutting forces, edge temperatures, finite element, modeling;
Increasing demands for higher rates of metal removal and productivity in modern manufacturing industry must be matched by enhancing the performance of cutting tools. Intense research on grade development by the tool industry has resulted in a continuous increase in grade performance to meet the demands of the manufacturing industry.
The plastic deformation of tools is one of the most important wear modes in metal cutting. Such deformation changes the geometry of the cutting edge, which often results in accelerated tool wear, increased cutting forces, risk of tool failure, vibrations and poor dimensional accuracy and surface finishes.
The high cost involved in obtaining machining data experimentally together with the opportunities to obtain a
better understanding of the basic mechanisms of the deformation process were the main motivations in the development of a methodology to study the plastic deformation of WC-Co cutting tools based on an experimental and numerical approach.
Empirical methods as well as analytical and numerical modelling have been applied to study different fundamental and technological aspects of the metal cutting process, such as chip formation, estimation of forces, stresses and temperatures and the prediction of wear and residual stresses on machined surfaces. Despite the significance of these phenomena, especially in continuous turning operations, rather few investigations concerning plastic deformation have been published. Often, the aim has been to predict the combinations of feed and speed that result in the plastic deformation of the cutting edge [1-5]; seldom has the plastic deformation and change in cutting edge geometry as such been modelled. One
© 2014 Published by Elsevier B.V. Open access under CC BY-NC-ND license. Selection and peer-review under responsibility of the International Scientific Committee of the 6th CIRP International Conference on High Performance Cutting
600 Anders Nordgren et al. / Procedia CIRP 14 ( 2014 ) 599 – 604
example of the latter is the work by Bell , who developed a 2D finite element (FE) model to describe the plastic deformation of tools in turning of steel (En24).
2.1. Tool materials
Two different cemented carbides were examined in this study, a fine-grained WC-10wt%Co alloy (A) and a medium coarse-grained WC-6wt%Co-alloy (B). The cemented carbides were of commercial grade, manufactured by standard production processes, i.e., pressing, sintering, edge treatment and finally deposition of a wear-resistant CVD coating. The coating consisted of an inner MTCVD Ti(C,N) coating, an intermediate alumina coating and an outer, thin TiN coating, exhibiting a total thickness of 7 μm. A CVD coating designed for machining steel was chosen for the present study because of its high wear resistance and the strong adhesion of the coating to the cemented carbide, which prevents the coating from flaking and the underlying substrate material from being exposed. Data for the cemented carbides and the coating are presented in Table 1.
Table 1. Data for cemented carbides and CVD-coating. Grain sizes are average values based on intercept measurements on scanning electron micrographs.
Grade Co-content [wt%]
WC grain size [μm]
HV3 Coating thickness [μm]
A 10 1 1620 7
B 6 2 1630 7
2.2. Creep and plasticity
In collaboration with KIMAB, Stockholm, a test procedure was developed for determining the high-temperature strength (creep and static strength) of cemented carbide in uniaxial, static compression. The procedure essentially follows SS-EN 24 506 Hardmetals – Compression test.
Creep implies time-dependent, non-elastic, plastic deformation [7-8] and is usually divided into three stages: a primary stage (transient stage, decreasing strain rate), a secondary stage (constant creep rate) and a tertiary stage (ultimately rupture). In the present investigation, the specimen was loaded with a constant stress, and the deformation was recorded as a function of time (creep curves).
For static, compressive strength testing [9-10], the specimen was subjected to an increasing stress at a constant deformation rate, and the resulting deformation was recorded as a function of applied stress (stress-strain-curves). In compressive strength testing at high temperature, creep deformation will contribute to the total deformation, and the material will relax due to time-dependent, plastic creep.
Creep and static strength were measured over the temperature range 800-1100◦C, a temperature range considered to capture cutting edge temperatures during continuous turning of steel. Static strength was tested over strain rate range of 10-4 to 10-2 s-1. The stress range examined
in the creep tests was 280-2400 MPa; in most cases, depending on the applied stress and temperature, the testing time was approximately 1800 seconds (30 minutes).
2.3. Turning tests
The deformation resistance of the CVD-coated cemented carbides was tested in ordinary longitudinal turning of quenched and tempered AISI 4340 steel bars, involving the engagement of the tool nose. The aim of these tests was determine the effect of tool grade (A vs B) and edge geometry (negative vs positive) on the tendency for plastic deformation and to use the performance relationships in subsequent modelling.
The workpiece material, cutting data and insert style were selected such that plastic deformation was the dominant wear mode and a relatively even distribution of edge deformation along the main cutting edge and tool nose was obtained. However, in this type of turning operation, completely even deformation along the cutting edge is not possible to achieve, and an increase in deformation from the depth of cut, along the edge, towards the tools nose is unavoidable. Figure 1 shows an example of a deformed cutting edge obtained from the turning tests.
Fig. 1. Flank view of a deformed cutting edge (flank land 0.38mm).
The quenched and tempered AISI4340 steel was machinability treated, i.e., the steel featured an inclusion pattern designed for increased machinability (to decrease tool wear and improve chip flow). The choice of workpiece material contributed to low tool wear and lack of interference from other wear phenomena during the tool deformation tests.
The cutting conditions were characterised by dry conditions (no coolant), high feed and a relatively high depth of cut. The insert styles used in the turning tests were TNMA220416 (rake angle -6o, clearance angle 6o) and TPUN220416 (rake angle +5o, clearance angle 6o), both insert styles with a flat rake face. Because the edge radius is known to affect the deformation of tools, inserts with a measured edge radius within a narrow range, approximately 40 μm, were used in the experiments.
During the turning tests, the machining was interrupted and the width of the flank land was measured every 30 seconds using a light optical stereo microscope. The measurements included both the flank land resulting fro